Brittle mixed-mode cracks between linear elastic layers
thesisposted on 2017-02-20, 10:22 authored by Joseph D. Wood
Original analytical theories are developed for partitioning mixed-mode fractures on rigid interfaces in laminated orthotropic double cantilever beams (DCBs) based on 2D elasticity by using some novel methods. Note that although the DCB represents a simplified case, it provides a deep understanding and predictive capability for real applications and does not restrict the analysis to a simple class of fracture problems. The developed theories are generally applicable to so-called 1D fracture consisting of opening (mode I) and shearing (mode II) action only with no tearing (mode III) action, for example, straight edge cracks, circular blisters in plates and shells, etc. A salient point of the methods is to first derive one loading condition that causes one pure fracture mode. It is conveniently called the first pure mode. Then, all other pure fracture modes can be determined by using this pure mode and the property of orthogonality between pure mode I modes and pure mode II modes. Finally, these 2D-elasticity-based pure modes are used to partition mixed-mode fractures into contributions from the mode I and mode II fracture modes by considering a mixed-mode fracture as the superposition of pure mode I and mode II fractures. The partition is made in terms of the energy release rate (ERR) or the stress intensity factor (SIF). An analytical partition theory is developed first for a DCB composed of two identical linear elastic layers. The first pure mode is obtained by introducing correction factors into the beam-theory-based mechanical conditions. The property of orthogonality is then used to determine all other pure modes in the absence of through-thickness-shear forces. To accommodate through-thickness shear forces, first two pure through-thickness-shear-force pure modes (one pure mode I and one pure mode II) are discovered by extending a Timoshenko beam partition theory. Partition of mixed-mode fractures under pure through-thickness shear forces is then achieved by using these two pure modes in conjunction with two thickness-ratio-dependent correction factors: (1) a shear correction factor, and (2) a pure-mode-II ERR correction factor. Both correction factors closely follow a normal distribution around a symmetric DCB geometry. The property of orthogonality between all pure mode I and all pure mode II fracture modes is then used to complete the mixed-mode fracture partition theory for a DCB with bending moments, axial forces and through-thickness shear forces. Fracture on bimaterial interfaces is an important consideration in the design and application of composite materials and structures. It has, however, proved an extremely challenging problem for many decades to obtain an analytical solution for the complex SIFs and the crack extension size-dependent ERRs, based on 2D elasticity. Such an analytical solution for a brittle interfacial crack between two dissimilar elastic layers is obtained in two stages. In the first stage the bimaterial DCB is under tip bending moments and axial forces and has a mismatch in Young s modulus; however, the Poisson s ratios of the top and bottom layers are the same. The solution is achieved by developing two types of pure fracture modes and two powerful mathematical techniques. The two types of pure fracture modes are a SIF-type and a load-type. The two mathematical techniques are a shifting technique and an orthogonal pure mode technique. In the second stage, the theory is extended to accommodate a Poisson s ratio mismatch. Equivalent material properties are derived for each layer, namely, an equivalent elastic modulus and an equivalent Poisson s ratio, such that both the total ERR and the bimaterial mismatch coefficient are maintained in an alternative equivalent case. Cases for which no analytical solution for the SIFs and ERRs currently exist can therefore be transformed into cases for which the analytical solution does exist. It is now possible to use a completely analytical 2D-elasticity-based theory to calculate the complex SIFs and crack extension size-dependent ERRs. The original partition theories presented have been validated by comparison with numerical simulations. Excellent agreement has been observed. Moreover, one partition theory is further extended to consider the blister test and the adhesion energy of mono- and multi-layered graphene membranes on a silicon oxide substrate. Use of the partition theory presented in this work allows the correct critical mode I and mode II adhesion energy to be obtained and all the experimentally observed behaviour is explained.
Loughborough University, Department of Aeronautical and Automotive Engineering.
- Aeronautical, Automotive, Chemical and Materials Engineering
- Aeronautical and Automotive Engineering
Publisher© Joseph D. Wood
Publisher statementThis work is made available according to the conditions of the Creative Commons Attribution-NonCommercial-NoDerivatives 4.0 International (CC BY-NC-ND 4.0) licence. Full details of this licence are available at: https://creativecommons.org/licenses/by-nc-nd/4.0/
NotesA Doctoral Thesis. Submitted in partial fulfilment of the requirements for the award of Doctor of Philosophy of Loughborough University.